Ultrasmall aqueous starch-capped CuS quantum dots with tunable localized surface plasmon resonance and composition for the selective and sensitive detection of mercury(ii) ions

Ultrasmall starch-capped CuS quantum dots (QDs) with controllable size were chemically fabricated in an aqueous medium. The phase of the CuS QDs was confirmed via X-ray diffraction (XRD), whereas the characteristic localized surface plasmon resonance (LSPR) peak in the near-infrared (NIR) region was measured using UV-Vis spectroscopy. Transmission electron microscopy and high bandgap analysis confirmed the formation of ultrasmall CuS QDs in the size range of 4–8 nm. CuS QDs have been used for the selective and sensitive detection of Hg2+ ions through colorimetric and spectroscopic techniques. The selective sensing of Hg2+ ions from various metal ions was detected via a remarkable change in color, damping in LSPR intensity, significant change in the Fourier-transform infrared spectra and X-ray photoelectron spectroscopic measurements. The mechanism of interaction between the CuS QDs and Hg2+ ions has been deeply explored in terms of the role played by the starch and the reorganization of sulfide and disulfide bonds to facilitate the access of Hg2+ ions into the CuS lattice. Finally, an intermediate Cu2−xHgxS nanostructure resulted in the leaching of Cu+ ions into the solution, which were further recovered and reused for the formation of fluorescent Cu2S nanoparticles. Thus, the entire process of synthesis, sensing and reuse paves the way for sustainable nanotechnology.


Introduction
Nature is colorful in the presence of light. Localized surface plasmon resonance (LSPR), the unique phenomenon that manifests in nanoscale materials, originates from the resonant interaction of free charge carriers with incident light. Traditional plasmonic nanoscale metals such as silver, 1 gold, 2 and copper 3 exhibit their corresponding LSPR in the visible region. LSPR observed in metal nanostructures can be slightly tuned in terms of size, shape, free electrons and the surrounding medium. In recent years, semiconductors exhibiting LSPR in the near or mid infra-red (IR) spectral region have drawn considerable attention due to their tunable plasmonic properties.
Semiconductor-plasmonic copper sulde (CuS) compounds are of interest due their key advantages such as stoichiometry, easy availability, tunable LSPR, low toxicity, recyclability and tunable band gap values from 1.2-2.0 eV. [4][5][6] CuS exists in different stable stoichiometries from copper rich chalcocite (Cu 2 S) to sulfur rich covellite (CuS) phases. In between these two stable phases, copper sulde exists in several stable and meta stable phases due to self-doped cation vacancies, oen represented as Cu 2Àx S, with very small x values. 7 Cu 2 S, acts as an intrinsic semiconductor, and exhibits no LSPR due to the absence of free carriers. However, stoichiometric CuS, acts as a p-type semiconductor because of Cu vacancies in its lattice and exhibits near infrared (NIR) LSPR in the wavelength range of 900-1200 nm due to the high concentration of free carriers. 6,7 From previous studies it is evident that the NIR LSPR property of CuS can be tuned by cation exchange, 8,9 varying the composition, size and crystal structure, 10,11 oxygen exposure and surface ligands, 12 temperature, 13 and phase transition. 14 Hence, the tunable optical phenomena of CuS open up the biological window in the NIR spectral region for its potential applications in drug delivery, 15 photothermal therapy 16 and therapeutics. 17 Insights into the cation-exchange reactions of CuS are fascinating and intriguing for the research community. Xie et al. reported that in a mild reducing environment, Hg 2+ ions exchange with CuS nanocrystals (NCs) to form HgS, Cu 2Àx S/HgS and Cu 2Àx S. 8 Wolf et al. compared the difference in damping, shiing and stability of LSPR in Cu 1.1 S nanoparticles, on incorporating Cu + and Ag + ions. 9 Stam et al. reported that Cu + ions intercalation leads to permanent phase transition from CuS to Cu 2 S NCs, whereas Li + ions interaction leads to reversible transition between CuS and CuLiS structures. 18 Recently, Liu et al. reported the reversible nanoscale interconversion from CuS to Cu 2 S nanocrystals (NCs) and vice versa. 14 It is well known that Hg 2+ ions have strong affinity towards sulfur ligands and sulfur anions (S 2À ) due to so-so interactions. 19,20 Hence, CuS nanostructures (NSs) with an interesting inherent cation exchange nature, unique optical properties and high affinity for S 2À ions, can be exploited to develop a selective, sensitive and rapid metal ion sensing platform.
Over the past few years, researchers have fabricated zerodimensional (0D), one-dimensional (1D), two-dimensional (2D) and three dimensional (3D) CuS NSs, such as nanodots, 21 nanocrystals, 8 thin lms, 22 nanotubes, 23 nanoplates, 24 nanosheets, 25 etc. These CuS NSs have been exploited for potential applications such as bioimaging, 26 photocatalysis, 27 nanoelectronics, 28 and theranostics. 29 Currently, there are various methodologies to fabricate CuS NSs, such as sonoelectrochemical, 30 hydrothermal, 30 solventless thermolysis, 30 mechanochemical, 31 microwave, 32 hot-injection, 14 and cationexchange reaction 33 methods. However, in most of these reports CuS NSs were prepared using expensive solvents, strong surfactants, and at high temperature and pressure. 34 Moreover, most of these methods were used to prepare CuS NSs with a size greater than 10 nm and unfortunately, that are insoluble or have low solubility in water. Moreover, insoluble CuS has practical limitations in the environmental eld, since sensing studies are carried out in water or organic solvents or a mixture of organic solvents/water. 35 As is known, the size reduction of nanomaterials into 0D quantum dots can cause signicant alteration in their physical and chemical properties due to a quantum connement effect. Shuang et al. synthesized stable water soluble amorphous and crystalline CuS QDs with average diameters of 2.7 and 3.3 nm, respectively, and exploited their properties in the antiproliferation of human cancer cells. 17 Therefore, it is vital to develop a simple route for the preparation of CuS QDs in water. Over the past few years, QDs have been widely used in the detection of transition metal ions 36 and heavy metals ions. 37 Based on their tunable optical properties, cation exchange reactions, sulfur rich nature and quantum size effect we hypothesize that CuS QDs might function as a novel Hg 2+ ion sensor, with distinct advantages over conventional analytical techniques and other nanomaterial-based sensors in terms of cost, solubility and environmental benignity.
Herein, we present a facile strategy for the synthesis of plasmonic CuS QDs in aqueous medium using a bottom-up approach. Starch, a natural biodegradable polymer, was used as both a reducing and capping agent. The size of the CuS QDs was controlled to below 10 nm by adjusting the reaction parameters. The as-prepared CuS QDs show the selective and sensitive sensing of Hg 2+ ions in water. Furthermore, we speculate a possible mechanism for the selective sensing of Hg 2+ ions using the CuS QDs. Moreover, the novel sensing platform provides multiple signal output in terms of color, composition, wavelength and intensity, enhancing its reliability in metal ion detection. Finally, from our reuse experiments, we found that Cu + ions released into the solution can be recovered to synthesize Cu 2 S NSs. Thus, the whole experimental process of synthesis, Hg 2+ sensing and reusability is an environmentally friendly process that can be used toward sustainable nanotechnology.

Materials and methods
All of the chemicals were of analytical grade with a purity of more than 98%, purchased from Merck Ltd. The aqueous solutions were prepared with double distilled water (DW) for all of the experiments.

Synthesis of CuS QDs
Briey, a transparent starch solution was rst prepared by mixing 2 g of starch in 250 ml of DW and the resultant turbid white solution was heated to 70-80 C under stirring for 15 min. Next, the hot transparent starch solution was used to prepare 1 mmol of CuCl 2 and Na 2 S solutions separately. Thereaer, the resultant starch mixed CuCl 2 and Na 2 S solutions were heated to 70 C under magnetic stirring for 10 min separately. Then, the as prepared hot Na 2 S-starch solution was added dropwise to a hot CuCl 2 -starch solution under vigorous stirring at 50 C, under a N 2 atmosphere. Aer cooling to room temperature, the as-prepared green solution of the CuS QDs was used for further instrumental characterization and experiments.

Results and discussion
The phase and morphology of the as-synthesized starch-capped CuS QDs were characterized by XRD, recorded using a PANalytical X'PERT PRO instrument equipped with an iron-ltered Cu-Ka radiation source (l ¼ 1.5406 A) in the 2q range of 20-80 , with a step size 0.02. The particle size of the CuS QDs was very small, therefore the sample was dried and calcined (at 110 C) and then the diffraction pattern was obtained. The phase and purity of the sample were conrmed according to the reference taken from JCPDS card no. 060464. The XRD patterns ( Fig. 1) show peaks corresponding to the (103), (006), (110) and (102) planes, indicating that the fabricated sample is hexagonal crystalline CuS QDs.
To investigate the nanostructure and topography, we used a FEI (model Tecnai F30) high resolution transmission electron microscope (HRTEM) equipped with a eld emission source operated at 300 KV to image the CuS QDs on a carbon-coated copper TEM grid. The TEM images (Fig. 2, panel A) show that the particles are spherical in morphology with an average size of around 4-8 nm. The particles are not well-dispersed but are fused together to form larger particles. The HRTEM image (Fig. 2, panel B) shows an interplanar spacing of 0.28 nm, which corresponds well to the (103) plane of CuS QDs. The selected area electron diffraction (SAED) pattern (Fig. 2, panel C) shows the polycrystalline nature of the CuS QDs. The particle size distribution (Fig. 2, panel D) of the CuS QDs shows that the average particle size is in the range of 4-8 nm.
The as-synthesized CuS QDs were further characterized by UV-Vis spectroscopy recorded on a UV-Vis spectrophotometer (Shimadzu, UV-1800) in the scan range of 190-1100 nm at a resolution of 2 nm. The UV-Vis absorption spectrum ( Fig. 3) of the CuS QDs shows an intense absorption peak in the UV and NIR region with a LSPR peak at approximately 975 nm. The phase purity, reaction parameters and particle size allowed us to tune the LSPR peak of the CuS QDs to 975 nm. However, CuS nanoparticles with a particle size in the range of 10-20 nm exhibited LSPR above 1000 nm. 16 The blue shi in the absorption spectra and LSPR peak positioning conrm a particle size of less than 10 nm. Moreover, it is known that LSPR is size dependent and red-shiing of peaks occurs with an increase in particle size. 11 Control of the optical properties of CuS QDs is fundamental for practical applications. With this in mind, we studied the effect of temperature on the optical behavior of CuS QDs. As the temperature was gradually increased, we observed a series of changes in the LSPR, namely a small blue-shi in the NIR LSPR  peak by 15 nm, a distinct change in the shape of the LSPR band, an increase in the LSPR absorption intensity and a narrowing and slight sharpening of the peak line width (Fig. 4). Moreover, these observations conrm that temperature can be used to tune the LSPR of the CuS QDs. In our previous work, we reported that temperature can be used to tune the surface properties of porous silica nanoparticles. 38 Therefore, the facile tunable LSPR and thermal stability of these CuS QDs opens the door to their use as light harvesting materials and in photothermal therapy.
It is imperative to highlight the energy band structure, which is the difference between the bottom of the conduction band (CB) and the highest occupied state in the valence band (VB). 39 From the absorption spectra, the direct band gap was measured using the following equation: where a is the absorption coefficient, hn is the photon energy, A is a constant, E g is the band gap, and the value of n is 2 for a direct transition. To calculate the direct band gap, we plotted a Tauc plot (Fig. 5) between hn and (ahn) 2 and from this the direct band gap of the as-synthesized CuS QDs was measured to be 5.08 eV. It is noteworthy that the band gaps calculated from temperature dependent studies were approximately equal to 5.0 eV. The band gap of the bulk material of CuS is 2.0 eV, while quantum connement can increase the band gap of bulk semiconductors by 1.0 eV. 10 In the case of CuS QDs, band gap variation depends on both quantum connement 30,40 and the Moss-Burstein effect. 30,41 A recent study showed that CuS NCs in the size range of 3-9.8 nm exhibited a band gap of 4.33 eV, due to a strong quantum connement effect. 42 Therefore, in the present work, the higher direct band gap obtained for the ultrasmall CuS QDs can be attributed to a quantum connement effect and these results further validate the size measurements seen in the TEM images. The overall results demonstrate the success in fabricating plasmonic CuS QDs in aqueous medium, with an ultrasmall particle size (4-8 nm), high thermal stability, tunable LSPR and high band gap. The green colored solution of the as-prepared CuS QDs indicated that they were well dispersed, homogenous and highly stable and showed no sign of aggregation, even aer one month of storage at room temperature in the dark. Next, 4 ml of starch-capped CuS QDs were taken up in a series of vials and then 0.5 ml of the abovementioned metal ion solution were added sequentially into each vial. The resulting solution mixture was shaken well and kept at room temperature for 10 min. We observed that the addition of Hg 2+ ions in CuS QDs resulted in a white colored solution, however, the addition of other metal ions shown no obvious color change (Fig. 6A). To gain insight into the selectivity of the CuS QDs for Hg 2+ ion detection, we further recorded UV-Vis spectra under the same conditions employed for the colorimetric detection. We observed that the LSPR of the CuS QDs at a wavelength of 975 nm disappeared and a new shoulder at approximately 330 nm appeared on addition of the Hg 2+ ions, whereas the LSPR was insensitive to the addition of the other metal ions ( Fig. 6B and C). Furthermore, the effect of the addition of different mercuric salts such as HgCl 2 , Hg(OAc) 2 and HgSO 4 to the CuS QDs also resulted in the appearance of a white colored solution (Fig. 7A) and the disappearance of the LSPR (Fig. 7B). Therefore, this nanosensor shows selective detection performance only for Hg 2+ ions rather than for other metal cations and anions. The sensitive detection performance of the proposed nanosensor was investigated by UV-Vis absorption spectroscopy. We monitored the LSPR of the CuS QDs at the 975 nm band feature  Paper in response to different concentrations of Hg 2+ ions. The LSPR intensity decreased continually with an increase in Hg 2+ ion concentration from 0 to 1000 mM (Fig. 8A), with a highly linear correlation coefficient (Fig. 8B).

Selective and sensitive detection performance of the CuS QDs
Colorimetric sensitivity is one of the key factors for a sensing system. Interestingly, we observed that the naked eye colorimetric responses of the CuS QDs were different against different concentrations of Hg 2+ ions (Fig. 9). It is clear that the addition of 10 mM of Hg 2+ ions changes the green colored CuS QDs to brown and upon a further increase in concentration, this brown color diminishes to pale brown and nally to white. Therefore, the limit of detection (LOD) for the Hg 2+ ions was 10 mM by eye.
Finally, to gain insight into the selectivity and sensitivity of the CuS QDs for Hg 2+ ion detection, we examined how the color and absorption spectra change with time upon the addition of Hg 2+ ions (500 mM). We observed a sequence of colorimetric change from green to white via brown, pale brown and pale white with an increase in time from 0-15 min (Fig. 10A). Simultaneously, UV-Vis absorption spectra were also recorded under the same conditions to those of the colorimetric responses. From the time-dependent UV-Vis absorption spectra, we observed a sequence of changes, namely a slight red shi with a gradual decrease in LSPR intensity, the disappearance of LSPR, and nally, the appearance of a new shoulder at approximately 340 nm (Fig. 10B). These results demonstrate that the nanosensor platform provides a multiple signal output in terms of color, intensity and wavelength.
It is well known that the target analyte is extremely toxic, therefore the detection limit is signicant. At a signal-to-noise ratio of 3, the limit of detection (LOD) for the Hg 2+ ions was estimated to be 1.95 mM. The limit of detection (LOD) of the proposed colorimetric sensing platform is compared with the other colorimetric sensors reported in the literature in Table 1.
In order to evaluate the practical applicability of the proposed colorimetric assay for the detection of Hg 2+ ions, various water samples, (TW: tap water from the IGNTU campus, RW: rain water harvesting pond, IGNTU campus, NRW: Narmada river, India) from regional sources were collected, ltered  and tested using a standard addition method. Unspiked water samples and samples spiked with 10 mM and 30 mM of Hg 2+ were prepared using various water resources. The UV-Vis absorption spectra of the CuS QDs remain almost invariable in the presence of various unspiked water samples (Fig. 11A-C). On the other hand, the Hg 2+ -spiked samples, spiked with either 10 or 30 mM of Hg 2+ , show red shiing with a decrease in the LSPR intensity. These characteristic changes in the absorption signatures validate that the Hg 2+ ions are denitely detected in various water samples. Furthermore, the 10 mM and 30 mM Hg 2+ spiked real water sample recovery rates are in the satisfactory range of 65-87% (Table 2). These results demonstrate that the colorimetric sensing platform can potentially be used for monitoring Hg 2+ ion content in drinking water.
Evolution: CuS to HgS via Cu 2Àx Hg x S NSs First, we compared two cases to explore the role of capping agent and particle size effect on the sensing of Hg 2+ ions by the CuS QDs. In the rst case, as stated in our present work, the assynthesized starch-capped CuS QDs exhibited sensing for Hg 2+ ions. Whereas, in the second case, a CuS precipitate was prepared using the same precursors and reaction conditions as described above in the synthesis of the CuS QDs without a starch solution. Interestingly, addition of Hg 2+ ions to the CuS precipitate showed no positive colorimetric and UV-Vis spectroscopic changes. These results further support and validate the effect of particle size and capping agent in the CuS QDs for the sensing of Hg 2+ ions. Next, we studied the interaction of Hg 2+ ions with the CuS QDs and speculated a possible interaction mechanism and sequential change in composition.
With the aim of investigating the evolution of Cu 2Àx Hg x S from CuS, we carried out X-ray photoelectron spectroscopy (XPS) analysis. For this purpose, the high resolution XPS data was collected by using a VG Microtech, model no ESCA 3000 equipped with an ion gun (EX-05) for cleaning the surfaces. The binding energy resolution was 0.1 eV. The XPS spectra reveal the oxidation state of Cu and S before evolution ( Fig. 12a and b) and Cu, Hg and S aer evolution (Fig. 12c-e). In the CuS QDs, the doublet peaks in the Cu 2p spectra centered at 933.4 and 954 eV were assigned as Cu 2+ 2p 3/2 and Cu 2+ 2p 1/2, respectively (Fig. 12a). [49][50][51] The presence of weak peaks at 944.2 eV can be attributed to satellite peaks of Cu 2+ . The feature in the S 2p spectra of CuS and Cu 2Àx Hg x S exhibited several interesting   Paper changes during the evolution of Cu 2Àx Hg x S from CuS. The S 2p spectra of the covellite CuS QDs feature doublet peaks at 161.8 and 163.2 eV (Fig. 12b) assigned to S 2p 3/2 and S 2p 1/2 respectively, which correspond to a sulde ion peak as a result of a Cu-S-Cu bonding conguration. 50,52,53 In comparison, for Cu 2Àx -Hg x S two doublet peaks were observed (Fig. 12d). The rst doublet peak for sulde ions has an S 2p 3/2 component at 161.9 eV and the other S 2p 1/2 component at 163 eV can be attributed to Cu-S bonding. 50 The second doublet peak for disulde ions shows an S 2p 3/2 component at 163.2 eV and another S 2p 1/2 component at 164.9 eV that appear as deconvoluted peaks (Fig. 12d), which can be attributed to a Cu-S-S-Hg bonding conguration. 50,52 The disulde ion bond energy appears at a higher binding energy than that of the sulde ion. The presence of another doublet for disulde bond energy corresponds to the highly nonstoichiometric copper decient sulde form. During this process there is a structural transformation and reorganization of the S atoms in the lattice, which facilitates the access of the Hg 2+ ions into the CuS lattice. Meanwhile, Cu + ions are released from the lattice and Hg 2+ ions occupy their position, resulting in the formation of Cu 2Àx Hg x S NSs. It is noted that Cu + ions released from the CuS lattice go into solution and can be recovered by ltration. The above proposal was conrmed from the Cu 2p XPS spectra of nonstoichiometric Cu 2Àx Hg x S (Fig. 12c). The XPS spectra conrmed the absence of the Cu 2+ state and the presence of a small doublet peak at Cu 2p 3/2 (932 eV) and Cu 2p 1/2 (952 eV), which   can be attributed to the Cu + state. The Hg 4f spectrum also exhibits a doublet feature due to spin orbit splitting and the resultant doublet peaks at 100.33 and 104.23 eV can be assigned to 4f 7/2 and 4f 5/2 , respectively (Fig. 12e), which correspond to the Hg 0 state and another doublet peak at 101.81 and 105.67 eV can be attributed to the Hg 2+ state. 54,55 Moreover, the Hg 0 state present on the surface can be attributed to the reducing effect of starch.
During the process of evolution, the CuS QDs exhibited ratiometric, colorimetric, wavelength and intensity responses to varying concentrations of Hg 2+ ions. The addition of a low concentration of Hg 2+ ions into the CuS QD solution brought about a colorimetric change (green to pale brown) and composition change (CuS to Cu 2Àx Hg x S and Hg x S NSs), which was evidenced by the strong red shiing and damping of the LSPR intensity. As the reaction proceeded, further exchange resulted in colorimetric change (pale brown to pale white) and composition change (Cu 2Àx Hg x S to Cu 2 S and HgS), and the formation of Cu 2 S was evidenced by complete disappearance of the LSPR and uorescence being exhibited in the presence of UV light. Interaction of the Hg 2+ ions favored the switching of the plasmonic CuS QDs to uorescent Cu 2 S NSs. Finally, a high concentration of Hg 2+ resulted in complete cation exchange and the resulting formation of HgS NSs, shown as a colorimetric change (pale white to milky white) and composition change (Cu 2 S to HgS & Hg 0 ). The formation of HgS was evidenced by the appearance of a new shoulder at 340 nm and the presence of Hg 0 was conrmed by XPS studies. 56 By controlling the addition of Hg 2+ ions, this method gives additional advantages to shi the LSPR to a desired wavelength and prepare Cu 2Àx Hg x S NSs. This is in agreement with previous studies on the transformation of CuS NCs into Cu 2 S via the incorporation of Cu + ions and CuS into Cu 2Àx S via the incorporation of Hg 2+ and Cd 2+ ions. 7,8 However, the reaction time for transformation in these previous works was 24 h. 7,8 In our present study, the starchcapped CuS QDs with unique properties reacted with Hg 2+ ions swily and the transformation of CuS to HgS occurred within 15 min.
Finally, the transformation of CuS to HgS was corroborated using Fourier-transform infrared (FT-IR) spectroscopy (Thermo Scientic iD7 ATR, Nicolet iS5) over a scanning range of 400 to 4000 cm À1 at a resolution of 4.0 cm À1 (Fig. 13). It can be observed that by comparing the FT-IR spectra of CuS and Cu 2Àx Hg x S, the characteristic vibrations at 3297 and 1623 cm À1 can be assigned to the vibrational and bending modes of OH groups, the peaks at 2360 and 1633 cm À1 can be assigned to the hydroxyl bending mode of water molecules, and the peak at 947 cm À1 can be assigned to the C-O-H bending vibration of starch, which exhibited a signicant change in transmittance aer the interaction with the Hg 2+ ions. The absorption bands between 1200 to 1000 cm À1 attributed to the C-O, C-C and C-O-H bending vibrations of starch, signicantly changed due the reduction process being carried out by the starch. 57 The vibrational peaks at 668 and 1074 cm À1 , assigned to the Cu-S stretching modes and asymmetric valence S]O vibration, 58,59 decreased aer the conversion of CuS to Cu 2Àx Hg x S, conrming the apparent rupturing of Cu-S and S]O bonds. Furthermore, the appearance of a new vibrational peak at 448 cm À1 , assigned to Hg-S stretching, 60 of considerable intensity, is an indication that some of the CuS was transformed into HgS. Thus, taken together, the UV-Vis, XPS and FTIR studies support our hypothesis that the CuS QDs were converted into HgS via Cu 2Àx Hg x S nanostructures as a result of cation exchange reactions and the reorganisation of the lattices.

Reuse experiment
Notably, the Cu + ions released into the solution from the exchanged lattices of CuS QDs were used in the formation of Cu 2 S NSs. In a typical recycling experiment, we collected and centrifuged the milky white solution. The supernatant solution containing Cu + ions was slightly warmed to 40 C and mixed with 1 mmol of hot starch mixed with a Na 2 S solution under a nitrogen atmosphere. The resultant mixture was le undisturbed and a brown colored solution was obtained. The UV-Vis absorption spectra of the resultant solution exhibited no peak or band in the NIR region. Furthermore, the brown solution showed photoluminescence, under a short UV light of 254 nm. As we know, Cu 2 S NSs exhibit no LSPR in the NIR region and the displaying of photoluminescence evidences the success of the recycling process. 18 Moreover, the results of this study expand our understanding on cation-exchange chemistry and provide a comprehensive approach to synthesize other familiar copper chalcogenides (CuSe, CuTe) and stoichiometric metal suldes (NiS, FeS and CoS) NSs and QDs.

Conclusions
We have presented a cost-effective and environmentally friendly approach to synthesize CuS QDs of controllable size in an aqueous medium. Cation exchange reactions, the reorganisation of sulde and disulde bonds, and the reducing properties of starch provide a unique set of tools to design a multi-output nanosensing platform for the detection of Hg 2+ ions in water. The metal ion exchange and sensing mechanism can be used to convert CuS to non-stoichiometric Cu 2Àx S NSs with the desired composition. Notably, the recycling experiments enabled us to synthesize Cu 2 S NSs, which further validated the environmentally friendly and sustainable nanotechnology approach. Overall, the CuS QDs have unique tunable optical properties and represent a rapid and feasible method for Hg 2+ assays.

Conflicts of interest
There are no conicts of interest.